Intercalant-independent transition temperature in ... - arXiv.org › publication › fulltext › Intercal... › publication › fulltext › Intercal...by R Zhang · 2017 · Cited by 65 — predicted to be tuneable by strain16 and electric field17, whereas surface ...
nd Astronomy, University of Manchester, Oxford Road, Manchester M13 9PL, United Kingdom 2 School of Earth, Atmospheric, and Environmental Sciences, University of Manchester, Oxford Road, Manchester M13 9PL, United Kingdom
Research on black phosphorus (BP) has been experiencing a renaissance over the last few years, after the demonstration that few‐layer BP exhibits high carrier mobility and a thickness‐ dependent band gap1,2,3,4,5. For a long time6,7, bulk BP is also known to be a superconductor under high pressure exceeding 10 GPa. The superconductivity is due to a structural transformation into another allotrope of phosphorous6,8 and accompanied by a semiconductor‐metal transition6. No superconductivity could be achieved for BP itself (that is, in its normal orthorhombic form) despite several attempts reported in the literature9,10,11,12. Here we describe successful intercalation of BP by several alkali metals (Li, K, Rb, Cs) and alkali‐earth Ca. All the intercalated compounds are found to be superconducting, exhibiting the same (within our experimental accuracy) critical temperature of 3.80.1 K and practically identical characteristics in the superconducting state. Such universal superconductivity, independent of the chemical composition, is highly unusual. We attribute it to intrinsic superconductivity of heavily‐doped individual phosphorene layers, while the intercalated layers of metal atoms mostly play a role of charge reservoirs. Bulk BP is the most thermodynamically stable phosphorus allotrope13 with a moderate direct bandgap (0.3 eV for bulk BP14, increasing to 2 eV for monolayer phosphorene2). Recent demonstrations of high mobilities3,5, quantum oscillations4, thickness‐dependent gap5 and field‐ effect transistors with high on‐off ratios15 using few‐layer BP has led to a strong wave of interest in this material in its quasi‐two‐dimensional form. Furthermore, the band gap of few‐layer BP has been predicted to be tuneable by strain16 and electric field17, whereas surface doping of few‐layer BP with potassium was found to result in a metallic state18. While the interest in semiconducting BP is focused on its promise for nanoelectronics and nanophotonics1, metallic BP was predicted to have sufficient electron‐phonon coupling to become a superconductor19.20. Metallic state and superconductivity in phosphorous were previously achieved in the 1960s (ref.6,7) by applying high pressure. The transition to the metallic state was shown to be associated with the structural transition from the orthorhombic to simple‐cubic crystal lattice, which actually means that the latter material was no longer BP but somewhat closer to white phosphorous that also has a cubic lattice8. The superconducting transition was found at 4.8K at 10 GPa and the transition temperature, Tc, could be further increased to 9.5K at 30 GPa (refs.6,7). The question whether it is possible to induce superconductivity in BP by other means has remained open. Recent experiments on electrostatically‐doped thin flakes of BP (ref. 21) did not find superconductivity, despite being able to 1
achieve carrier concentrations well above 1013 cm‐2, sufficient to induce superconductivity in, e.g., electrostatically‐doped MoS2 (ref.22). There were also several attempts to obtain intercalated compounds of BP by reacting it with alkali metals9 (K, Cs and Li), iodine10, and AsF5 (ref. 11) and by electrochemical lithiation12. No stable intercalation compounds could be achieved in either of these studies, and no superconducting response was reported or discussed. To overcome the problem of disintegration of BP crystals when in contact with highly reactive vapours of alkali metals, we have employed an alternative technique of liquid ammonia intercalation23,24. This allowed us to achieve successful intercalation of BP crystals with several alkali and alkali‐earth metals: lithium (Li), potassium (K), rubidium (Rb), caesium (Cs) and calcium (Ca). All our intercalation compounds show superconductivity with Tc of 3.8 K, the same value within our experimental accuracy of 0.1 K. We emphasise that Tc does not depend on the intercalating metal, which indicates that the superconductivity is an intrinsic property of electron‐doped phosphorene (individual layers of black phosphorus), as described below.
Figure 1| Structure and composition of pristine and intercalated black phosphorus. (a, b) Schematic structure of black phosphorus before (a) and after (b) intercalation. ‘P’ stands for phosphorus atoms and ‘M’ represents intercalating metals Li, K, Rb, Cs or Ca. The shown positions of metal atoms correspond to the results of first‐principle calculations20,25,26. Those suggested that the adjacent phosphorene layers should slide with respect to each other, effectively changing the